Irreversible Property Changes of Small Loblolly Pine Specimens Heated in Air, Nitrogen, Or Oxygen
Keywords:Pinus taeda, heating, thermal degradation, strength loss, stiffness loss, hygroscopicity, hydrolysis, oxidation
The objective of this research was to characterize the roles played by atmospheric oxygen and wood moisture in the thermal degradation of loblolly pine as measured by selected physical and mechanical properties. These two factors relate, respectively, to the oxidation and hydrolysis reactions that comprise the total degradation reaction.
Small clear specimens were individually heated at 150 C from 1 to 16 hours in airtight cylinders, which were flushed with oxygen, nitrogen, or air prior to being to sealed. Measured properties were rellectance, specific gravity, hygroscopicity, and the moduli of rupture and elasticity in bending.
Property values generally exhibited a decrease with increasing exposure time. The properties can be ranked from most-to-least degraded as follows: relfectance, modulus of rupture, hygroscopicity, modulus of elasticity, and specific gravity. The degradation of these properties was not adequately described by first-order reaction kinetics, Instead, a nonlinear equation was used, which accurately described the data and still reflected a rate controlled process.
The rate of property loss was accelerated by the presence of wood moisture, with the exception of residual hygroscopicity. The greatest decrease in property due to the presence of wood moisture occurred with reflectance. The degradation of modulus of rupture and modulus of elasticity was directly related to the amount of wood moisture present.
The apparent role of oxygen in total thermal degradation depended on specimen moisture content. The influence of oxygen on the the degradation process was apparent for specimens heated in the oven-dry condition. When moist specimens were heated, however, losses caused by hydrolysis overshadowed oxygen-dependent degradation. Oxygen-dependent degradation was most visible for moduli of rupture and elasticity, and, to a lesser degree for reflectivity. No effect due to the presence of oxygen could be discerned for residual specific gravity and hygroscopicity.
Hillis, W. E. 1975. The role of wood characteristics in high temperature drying. J. Inst. Wood Sci. 7(2):60-67.nKoch, P. 1971. Process for straightening and drying southern pine 2 by 4's in 24 hours. Forest Prod. J. 21(5): 17-24.nKoch, P. 1976. Strength of southern pine lumber dried at high temperatures. Proc. Research Conference on High-Temperature Drying Elfects on Mechanical Properties of Softwood Lumber, Madison, WI. Pp. 38-49.nMcGinnis, G. D., W. W. Wilson, and C. J. Bierman. 1984. Biomass conversion into chemicals using wet oxidation. Pages 89-109 in Don Wise, ed. Byconversion systems. CRC Press, Boca Raton, FL.nMacLean, J. D. 1951. Rate of disintegration of wood under di Herein heating conditions. Am. Wood Preservers' Assoc. Proc. 47:155-168.nMacLean, J. D. 1953. Effect of steaming on the strength of wood. Am. Wood Preservers' Assoc. Proc. 49: 88-112.nMacLean, J. D. 1954. Effect of heating in water on the strength properties of wood. Am. Wood Preservers' Assoc. Proc. 50:253-280.nMacLean, J. D. 1955. Effect of oven-heating and hot-pressing on strength properties of wood. Am. Wood Preservers' Assoc. Proc. 51:227-250.nMillett. M. A., and C. C. Gerhakds. 1972. Accelerated aging: residual weight and flexural properties of wood heated in air at 115° to 175° Wood Sci. 4(4): 193-201.nPrice, E. W., and P. Koch. 1980. Kiln time and temperature affect shrinkage, warp, and mechnical properties of southern pine lumber. Forest Prod. J. 30(8):41-47.nSAS Institute: Inc. 1985. SAS User's Guide: Statistics, Version 5 Ed. SAS Institute Inc., Cary, NC.nSkaar, C. 1976. Efect of high temperatures on the rate of degradation and reduction in hygroscopicity of wood. Proc. Research Conference on High-Temperature Drying Effects on Mechanical Properties of Softwood Lumber, Madison, WI. Pp. 113-127.nStamm, A. J. 1956. Thermal degradation of wood and cellulose. Ind. Eng. Chem. 48(3):413-417.nStamm, A.J., H. K. Burr, and A. A. Kline. 1955. Heat-stabilized wood (Staybwood). USDA Forest Serv., Forest Prod. Lab. Rep. No. 1621.nYao, J., and F. Taylor. 1979. Effect of high-temperature drying on the strength of southern pine dimension lumber. Forest Prod. J. 29(8):49-51.n
The copyright of an article published in Wood and Fiber Science is transferred to the Society of Wood Science and Technology (for U. S. Government employees: to the extent transferable), effective if and when the article is accepted for publication. This transfer grants the Society of Wood Science and Technology permission to republish all or any part of the article in any form, e.g., reprints for sale, microfiche, proceedings, etc. However, the authors reserve the following as set forth in the Copyright Law:
1. All proprietary rights other than copyright, such as patent rights.
2. The right to grant or refuse permission to third parties to republish all or part of the article or translations thereof. In the case of whole articles, such third parties must obtain Society of Wood Science and Technology written permission as well. However, the Society may grant rights with respect to Journal issues as a whole.
3. The right to use all or part of this article in future works of their own, such as lectures, press releases, reviews, text books, or reprint books.